abstract. The stable form of Ti02 above 400° C. was found to be rutile with a melting point of 1,825° C. ... hydroxide is dehydrated by heating to a temperature below about. 900°. l ... that anatase can exist in two forms, a and /?, which are in equilibrium at 642°, while ... preparations to contain 100.0 percent Ti02 . Brookite was ...
Department of Commerce, Bureau of Standards
RESEARCH PAPER RP619 Part of Bureau of Standards Journal of Research, Vol. 11, November 1933
PHASE EQUILIBRIA IN THE SYSTEMS Ti0 Ti0 2 ~Al 2 By
Ti0 2 -Si0 2
E. N. Bunting
abstract stable form of Ti0 2 above 400° C. was found to be rutile with a melting point of 1,825° C. It forms no compounds with Si02, but gives a eutectic with 89.5 wt. percent Si0 2 at 1,540° C. With A1 2 3 a compound Ti 2 .A1 2 3 is formed, melting at 1,860° C. This compound forms a eutectic with Ti0 2 at 15 wt. percent A1 2 3 and 1,715° C, and a second eutectic with A1 2 3 at 62 wt. percent A1 2 3 and 1,850° C. Several low melting fluxes with nonvolatile acid radicals are described.
CONTENTS Page I.
719 719 722 724
The system Ti0 2 III. The system Ti0 2 -Si0 2 IV. The system Ti0 2 -Al 2 3 II.
Titanium dioxide resembles silica in chemical behavior and has found use in the ceramic arts as an opacifying material in enamels and glass. Its high index of refraction might be of value in the preparation of special glasses, if clear titanate glasses can be made. The high melting point of titania makes it useful as a refractory, although it cannot compete at present with the cheaper refractories. However, complete information regarding its value to the ceramic industry can only be gained by a thorough investigation of its reactions with the ceramic materials. The present work deals with the forms of titanium dioxide and its reactions with silica and alumina. II.
Titania is found in nature in three crystalline forms, namely, anatase, brookite, and rutile. Anatase is formed whenever titanium hydroxide is dehydrated by heating to a temperature below about 900°. l It is reported in the literature 2 3 that brookite was obtained by laboratory reactions at temperatures between 800° and 1,040°. However, the present work has shown that brookite changes to rutile below this temperature region in the presence of a suitable flux, or mineralizer, and that rutile is formed from anatase above 400°. 1
All temperatures are given in degrees centigrade. P. Hautefeuille, Bull. soc. chim., vol. 5, p. 588, 1863;
rend., vol. 57, p. 148, 1863; vol. 59, p. 188,
Ann. chim. phys. A, vol. 4, p. 131, 1865. A. Daubree, Ann. mines, vol. 16, p. 129, 1849; Phil. Mag., vol.
1864; vol. 90, p. 868, 1880; 3
vol. 57, p. 307, 1854;
9, p. 315, 1855; Edinburgh Phil. Jour., rend., vol. 29, p. 227, 1849; vol. 30, p. 383, 1850; vol. 39, p. 153, 1853.
of Standards Journal oj Research
Conditions of stability for the natural minerals, without the presence of a mineralizer, have been studied by A. Schroder. 4 He found that anatase can exist in two forms, a and /?, which are in equilibrium at 642°, while at 915° ±15° the a-anatase changes irreversibly to
He also found that brookite changes to r utile with a velocity that is an exponential function of the temperature, the change not being measurable below about 650°. Rutile was not changed to the other forms at any temperature. His results were based on changes in prism angles and densities. Anatase was prepared from TiCl/ by hydrolysis with distilled water, the resulting hydroxide being dried at about 400°. On heating rutile.
* A. Schroder, Zeit. Exist., vol 66, p. 493, 1928, and vol. 67, p. 485, 1928. The TiC-U was prepared from commercial TiCU by S. T. Schicktanz by fractional distillation through a 20-plate still, only the middle fractions being used.
The Systems Ti0 2 Ti0 2 -Si0 2 and Ti02 -Al 2
above 1,000°, pure rutile was obtained. Analyses showed these preparations to contain 100.0 percent Ti0 2 Brookite was used in the form of finely powdered natural mineral, purified somewhat by repeated extractions with hot hydrochloric acid. For the experiments described below it was necessary to find suitable low melting fluxes in which Ti0 2 would dissolve but with which not all of the sample would react. The vanadates and dichromates were found to be suitable, and the fusion temperatures of some mixtures were determined by the cooling and heating curve method, using about 50 g of stirred material. Melting points of commercial 3 NaV0 3 and LiV0 3 each containing about 1 percent of carbonate, .
were found to be 527°, 588°, and 599°, respectively. The minimum melting temperature for KV0 3 -NaV0 3 mixtures is 480°, at 85 wt. percent KV0 3 and for NaV0 3 -LiV0 3 this temperature is 556°. A minimum melting temperature in KV0 3 -NaV0 3 -LiV0 3 is at 461°, with a composition close to 77.6 wt. percent KV0 3 -13.4 percent NaV0 3 The addition of 10 percent of V 2 5 to this mix9.0 percent LiV0 3 ture gives one which is partially molten at 445°. The minimum melting temperature for mixtures is 310°, in the 2 Cr 2 7 -NaV0 3 neighborhood of 25 wt. percent NaV0 3 A convenient mercury-vapor bath which was used for heating over long periods at temperatures between 300° and 380° is shown in figure 1. It is made of pyrex glass and is filled with nitrogen at a pressure determined by the temperature desired. With changes in room temperature of not more than 3°, the temperature of the bath will remain constant to within about 1°. A 200- to 300-watt heater serves to vaporize the mercury. ,
Treatments given anatase seeded with brookite and rutile
Do Do Do Do Do Do
NaV0 +KV0 +LiV0 3
Do Do Do
NaV0 +K Cr207— 3
Do Do Do
NaV0 +HoO 3
5 to 10
700 725 750 775 790 800 840 795 725 575 425 465 500 515 550 550 525 400 350 350
Hrs. 24 24 24 24 24 24 24 24 24 24 168 125 48 24 24 24 24 600 700 90
Do. Do. Do. Do. All changed Do. Do. Do. Do.
Do. Do. Do. Do. Do. Do.
percent rutile. present.
In the presence of mineralizers anatase and brookite will change to much lower temperatures than those reported by Schroder, as shown in tables 1 and 2. The rate at which anatase is changed to rutile depends upon the flux present as well as upon the temperature. Table 3 shows the treatments given rutile, none of which resulted in changing it. rutile at
of Standards Journal of Research
— Treatments given
brookite seeded with anatase
NaV6 +KV03+LiV0 3
— Treatments given
350 425 475 525 320
Cr 2 07
Cr 2 07
Do. Do. All rutile. No change.
anatase and brookite
NaV03+K Cr 07 NaV03+KV03+LiV0
Temper- Duration ature
Na W04 Do Do Do Do Do Do NaVCh
90 24 24 24 1,700
rutile seeded with
725 840 900 950 1,000 1,100 1,200 1,400 600 500 475 425 350 350 325
24 24 24 24 24 24 24 24 24 168 168 24 90 700 640
Do. Do. Do. Do. Do. Do. Do. Do. Do. Do. Do. Do. Do. Do.
Identification of the crystal forms of the Ti0 2 was made by X-ray spectrograms 6 of the powdered material after all the mineralizer had been thoroughly removed by repeated washings with water, dilute solutions of HC1, and aqueous ammonia. Samples of natural brookite and rutile obtained from the National Museum and anatase prepared artificially were used as identifying standards. All heatings were made in platinum crucibles in an electrically heated tube furnace controlled to ±1°. The data indicate that if there is a temperature where rutile is in stable equilibrium with anatase or brookite, it must be below 400°. The melting point of rutile 7 has been reported as 1,560° to 1,980°. Kecent determinations by Wartenberg are 1,850° 8 and 1,825°. 9 The melting point, as determined in a hole in an iridium button heated by high-frequency induction 10 was found to be 1,825°. Although this determination can be duplicated within ±5°, a correction of 10° to 20° should be added, as the material would not be visible under exact black body conditions. The white color of anatase changes to a light tan when it changes to rutile, and the color darkens as the rutile is heated to higher temperatures, becoming blue-black on melting. III.
The only previous work on this system is that reported by Rieke, 11 who observed the fusion of cones of mixtures heated in a carbon resistance furnace. Considerable reduction of the Ti0 2 must have occurred, 6 The X-ray spectrograms were made by the metallurgical division of this Bureau. 7 See J. W. Mellor, A Comprehensive Treatise on Inorganic and Theoretical Chemistry, vol. 7, Green, and Co., New York and London. 1927. 8 Wartenberg and Gurr, Z. anorg. Allgem. Chem., vol. 196, p. 374, 1931. s Wartenberg and Prophet, Z. anorg. allgem. Chem., vol. 208, p. 369, 1932. 10 See Bunting, B. S. Jour. Research, vol. 4, p. 131, 1930. ii R. Rieke, Sprechsaal, vol. 41, p. 405, 1908.
— The Systems Ti0 2 Ti02 -Si0 2> and Ti0 2 -Al 2
or else he used impure Ti0 2 as he found the melting point to be near cone 27, or about 1,600°. Under the reducing conditions in a carbon furnace it is not possible to obtain the correct temperatures for the fusion of binary mixtures containing reducible oxides. ,
ground quartz crystals (99.7 percent Si0 2 ) and rutile Ti0 2 ) were made by wet grinding in an agate mortar. Thorough mixing was further obtained by three fusions, in the oxyhydrogen flame, and intermediate grindings. All mixtures containing not over 20 wt. percent of Ti0 2 were heated in a platinum capsule in a rhodium wire resistance furnace for two hours or more before Mixtures of (100.0 percent
T i0 1700
Lie I u
Phase diagram for
WEIGHT PERCENT the
system Ti0 2 -Si0 2
quenching. The phases present in the quenched material were determined with a petrographic microscope. The fusion of mixtures containing over 20 percent Ti0 2 was observed in the iridium button. 12 All temperatures were determined on a disappearing filament optical pyrometer 13 and are probably correct to within 10°. The results are shown in table 4 and figure 2. X-ray spectrograms of mixtures containing 40, 50, 57, 65, 70, and 80 wt. percent Ti0 2 which were quenched from 1,720°, snowed only the presence of rutile crystals. The data show that no compounds are formed and that the eutectic between rutile and cristobalite occurs at 10.5 wt. percent Ti0 2 and 1,540° ±10°. ,
» See 13
Recently calibrated by the pyrometry section of this Bureau.
Bureau of Standards Journal Table
Ti0 2 weight
Ti0 2 -Si02 mixtures Ti0
1,670 1,665 1,580 1,575 1,540 1,605 1,600 1,540
+ cristobalite. All glass. Glass + cristobalite. Cristobalite + rutile. All glass. Glass + rutile. Glass
All glass. Glass rutile. All glass. Glass rutile. All glass. Glass rutile.
1,625 1,620 1,680 1,675 1,725 1,715
+ + +
Cristobalite -f rutile.
The fusion of mixtures of Ti0 2 and A1 2 3 was observed in the iridium button with the optical pyrometer. The observed fusion temperatures are probably correct to within 25°, since exact black body conditions are not present. Duplicate determinations on small pieces weighing a few milligrams can, however, be checked within about 10°. Determinations on mixtures which are not eutectics or compounds will give temperatures too low, as the mixture will appear to be all melted while some crystals may still be present. Mixtures were prepared from finely ground rutile (100.0 percent Ti0 2 ), and A12 3 (99.95 percent) obtained by igniting aluminum nitrate. The aluminum nitrate was prepared by dissolving aluminum (99.95 percent) 14 in nitric acid of reagent quality and evaporating to dryness in a platinum dish. When ignited to 900°, the A1 2 3 contained subniwhile after ignition at 1,200° trates equivalent to 0.22 percent 2 5 15 only 0.04 percent was found. No determinable quantity of 2 5 combined nitrogen could be found in the fused A1 2 3 The mixtures were mixed wet and formed into sticks which were prefused in the oxy-hydrogen flame, using an excess of oxygen to minimize the formation of lower oxides of titanium. The compositions of the mixtures with their fusion temperatures are given in table 5 and figure 3. The data obtained by Wartenberg and Reusch 16 are also shown. They interpret their data to indicate the formation of the compound 2Ti0 2 .Al 2 3 although they might just as well indicate the compound Ti0 2 .Al 2 3 The present data indicate the formula Ti0 2 .Al 2 3 for the compound. As additional evidence, X-ray spectrograms were made of fused mixtures corresponding to these two formulas. The spectrograms showed that the compound is Ti0 2 .Al 2 3 as no rutile lines were present in the fusion of this composition, while the spectrogram of the 2Ti0 2 .Al 2 3 "mixture consisted only of the lines of the Ti0 2 -Al 2 3 mixture plus those of rutile. 17 The melting point of Ti0 2 .Al 2 3 is about 1,860°,
Analysis by J. A. Scherrer of the Chemistry Division, Bureau of Standards, Analysis by H. A. Buchheit of the Chemistry Division, Bureau of Standards. Wartenberg and Reusch, Z. anorg. allgem. Chem., vol. 207, p. 10, 1932. 17 A microscopic examination by Herbert Insley of the mixture with the composition TiOa.AbOa which had been fired in the oxy-hydrogen flame showed it to be completely crystalline and to consist wholly of one phase. The crystals had the following optical properties: 7Li=2.015±0.01,aLi=1.975=b0.01, biaxial (— ), medium 2V. Extinction parallel with a pronounced prismatic development and good cleavage parallel to a. Pleochroism is strong with a=nearly colorless, 7= deep bluish green. Thick crystals are so deeply colored in th9 y direction as to be almost opaque. 14
—— The Systems Ti02 Ti02 -Si02 and Ti02 -Al2 Oz
and iff forms a eutectic with Ti0 2 at 15 wt. percent A12 3 and and a eutectic with A12 3 at 62 wt. percent A1 2 3 and 1,850°. r
War teniDerg a
r eusc h